Delft University of Technology
To fold or not to fold?
An exploration of deployable porous biomaterials for the treatment of large bone defectsBobbert, F.S.L. DOI 10.4233/uuid:ac6113f5-9777-49a3-b559-f14554ffc210 Publication date 2021 Document Version Final published version Citation (APA)
Bobbert, F. S. L. (2021). To fold or not to fold? An exploration of deployable porous biomaterials for the treatment of large bone defects. https://doi.org/10.4233/uuid:ac6113f5-9777-49a3-b559-f14554ffc210
To cite this publication, please use the final published version (if applicable). Please check the document version above.
Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy
Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.
This work is downloaded from Delft University of Technology.
To fold or not to fold?
To fold or not to fold?
An exploration of deployable porous biomaterials for the treatment of large bone defects
ter verkrijging van de graad van doctor aan de Technische Universiteit Delft,
op gezag van de Rector Magnificus, Prof.dr.ir. T.H.J.J. van der Hagen, voorzitter van het College voor Promoties,
in het openbaar te verdedigen op vrijdag 9 juli 2021 om 12:30 uur.
Françoise Siu Lin BOBBERT
Master of Science in Biomedical Engineering, Technische Universiteit Delft, Nederland,
Dit proefschrift is goedgekeurd door de promotor. Samenstelling promotiecommissie bestaat uit:
Rector magnificus, voorzitter
Prof.dr. A.A. Zadpoor Technische Universiteit Delft, promotor
Prof.dr.ir. J.L. Herder Technische Universiteit Delft
Prof.dr. E. Karana Technische Universiteit Delft
Prof.dr. E.B. Wolvius Erasmus MC
Dr. J. Jeffers Imperial College London
The research leading to these results has received funding from the European Research Council under ERC agreement no. .
Keywords: bone tissue engineering, deployable structures, biomaterials, origami, kirigami Printed by: Gildeprint
Copyright © 2021 by F.S.L. Bobbert ISBN 978-94-6419-248-3
1.2 Bone structure and the remodeling process...2
1.3.1 Biomaterial architecture...3
1.3.2 Biomaterial surface...4
1.4 Minimally invasive surgery...4
1.5 Deployable structures...4
1.5.1 Rigid assemblies...5
1.5.2 Elastic deformation...5
1.5.3 Plastic deformation...5
1.6 Problem statement...5
1.7 Aim and research questions... 6
1.8 Thesis outline...6
2 The effects of the bone substitute architecture on the bone regeneration
2.2 Pore size and porosity...16
2.2.1 Seeding efficiency...16
2.2.2 Cell viability...17
2.2.3 Cell migration...20
2.2.4 Cell alignment and morphology...20
2.2.5 Cell proliferation...21
2.2.6 Cell differentiation...21
2.2.7 Blood vessel formation...22
2.2.8 Tissue formation and mineralization...23
2.2.9 Structure of the new bone...23
2.3 Pore shape and fiber orientation...24
2.3.2 Cell migration...25
2.3.3 Cell alignment and morphology...25
2.3.4 Cell proliferation...25
2.3.5 Cell differentiation...28
2.3.6 Blood vessel formation...28
2.3.7 Tissue formation and mineralization...28
2.3.8 Structure of the new bone...29
2.4 Surface topography and chemistry...30
2.4.1 Seeding efficiency...30
2.4.2 Cell alignment and morphology...30
2.4.3 Cell proliferation...31
2.4.4 Cell differentiation...31
2.4.5 Tissue formation and mineralization...31
2.5 Structure stiffness...34
2.5.1 Seeding efficiency...34
2.5.2 Cell viability...35
2.5.3 Cell alignment and morphology...35
2.5.4 Cell differentiation...35
2.5.5 Tissue formation and mineralization...38
2.6 Discussion and conclusion...38
3 Rigid porous biomaterials...49
3.2 Materials and methods...51
3.2.1 Porous biomaterial design and manufacturing...51
3.2.2 Porous biomaterial morphology...52
3.2.4 Mechanical tests...56
3.3.1 Morphology of the porous biomaterials...57
3.3.2 Permeability values...57
3.3.3 Mechanical tests...60
3.4.1 Morphological properties...65
3.4.2 Quasi-static mechanical properties...68
3.4.3 Fatigue behavior...69
3.4.5 Design implications...71
4 Deployable non-assembly mechanisms...79
4.2 Materials and methods...81
4.2.1 Design...81 4.2.2 Manufacturing...84 4.2.3 Mechanical tests...85 4.3 Results...86 4.3.1 Change in dimensions...86 4.3.2 Mechanical tests...86 4.4 Discussion...89 4.4.1 Deployability...90 4.4.2 Mechanical performance...91 4.4.3 Future work...93 4.5 Conclusions...93 References...94
5 Multi-stable structures...99 References...109
6 Deployable structures folded from a flat state...113
6.2 Materials and methods...116
6.2.3 Assembly of cubes...118
6.2.5 The Russian doll (Matryoshka) principle...119
6.2.6 Change in dimensions between the deployed and retracted structure...119
6.2.7 Mechanical test...119
viii 6.3.2 Mechanical tests...121 6.3.3 Micropatterns...123 6.4 Discussion...125 6.4.1 Deployability...126 6.4.2 Mechanical performance...126
6.4.3 Surface nanopatterns and other bio-functionalities...127
7 General Discussion and conclusion...135
7.1 Main findngs of this thesis...136
7.2 Manufacturing techniques...139
7.2.1 Selective laser melting...139
7.2.2 Fused deposition modeling...139
7.2.3 Laser micromachining...140 7.3 Deployability...140 7.3.1 Non-assembly mechanisms...140 7.3.2 Multi-stable structures...141 7.3.3 Deployable cubes...141 7.4 Mechanical performance...142 7.4.1 Load-bearing locations...142
7.4.2 Rigid porous biomaterials...142
7.4.3 Deployable non-assembly mechanisms...142
7.4.4 Multi-stable structures...143
7.4.5 Deployable cubes...143
7.5 Load-bearing capacity of the various designs...143
SummaryWithout our musculoskeletal system, which consists of bones, joints, and muscles, we would not be able to live. Our bones are responsible for the protection of our organs, the support of our body, and they enable our mobility. Therefore, it is important to keep them healthy. This is done by cells who repair small cracks and fractures caused by our daily activities through continuous remodeling of the skeleton. However, severe bone damage and defects can occur, for example, due to trauma (e.g., car accidents) and bone tumor resection. In this case, the defects are too large for the cells to repair and surgical intervention is required to support the bone regeneration process. Bone substitutes or porous biomaterials are used to fill these defects to help the cells to regenerate the bone.
Bone substitutes require implantation via open surgery due to their large dimensions and rigidity. This causes great damage to the body, which results in a long recovery time for the patient and increases the risk of infections. To reduce the invasiveness of the implantation process, minimally invasive surgery (MIS) could be used. MIS techniques make it possible to perform surgical treatments through specific minimally invasive tools that are inserted into the body through small incisions. In order to make minimally invasive implantation possible, the dimensions of porous biomaterials should be reduced to fit through these small incisions.
In addition, it has been demonstrated that the bone regeneration process can be optimized and infections could be prevented by applying precisely controlled nanopatterns to the surface of bone substitutes. However, surface patterning techniques can only be applied to flat surfaces. Therefore, it is not possible to apply surface patterns to the inner surfaces of three-dimensional porous structures, such as those fabricated through 3D printing techniques.
To resolve these two issues, biomaterials could be made deployable and be folded from flat sheets to simultaneously enable the use of MIS and surface patterning techniques. Because neither deployable nor foldable biomaterials have been developed before, the aim of this thesis is to explore the feasibility of making porous biomaterials deployable and foldable from a flat state.
In order to understand the important architectural parameters of porous biomaterials and their effect on the bone regeneration process, a literature review was conducted in Chapter 2.
In Chapter 3, rigid metallic porous biomaterials based on four different types of minimal surfaces were designed using a three-dimensional computer models. Computer models allow for the design of porous biomaterials with the desired properties for the application as bone substitutes. These computer models were used to manufacture the rigid porous
printing) technique to build metal objects. This enabled us to evaluate the mechanical (i.e., quasi-static mechanical properties and fatigue behavior) and mass transport properties of solid free-form fabricated porous biomaterials.
Although the porous structures presented in Chapter 3 offer a unique combination of mechanical and mass transport properties, they are not suitable to be implanted using MIS procedures. Therefore, a first step towards deployable metallic biomaterials is made in Chapter 4. This chapter presents deployable non-assembly mechanisms, which were manufactured using SLM. Different geometries consisting of revolute joints, wavelike elements, and rigid rods were assembled into structures that could be deployed and retracted by applying compressive or tensile forces to their proximal and distal vertices.
The revolute joints in the deployable non-assembly mechanisms presented in Chapter 4 complicate the design of deployable porous biomaterials. Therefore, they were eliminated from our deployable designs presented in Chapter 5. Bi-stable elements were printed using fused deposition modeling (FDM). The bi-stable elements were combined in various ways to make multi-stable structures that can be deployed in different ways.
Although the multi-stable structures developed in Chapter 5 were deployable, their three-dimensional design does not allow for the application of surface patterning techniques. In Chapter 6, the knowledge gained from this study was used to develop deployable and foldable structures. FDM and laser micromachining were used to create three-dimensional deployable cubes. Due to the flat state of the laser-cut metal sheets, it was possible to apply micro-patterns to their surfaces. Moreover, the metal sheets could be folded into three-dimensional deployable configurations.
Chapter 7 summarizes the main findings of the thesis and tries to formulate succinct answers to the primary and secondary research questions presented in Chapter 1. Additionally, recommendations for future research are provided and alternative applications are proposed.
Overall, the work covered by this thesis is the first step towards the development of deployable porous biomaterials, which can be folded from a flat state. We hope that our designs provide inspiration for the further development of such biomaterials and for making them available for the treatment of large bone defects. Such biomaterials should be also compatible with MIS techniques and allow for the application of precisely-controlled surface nanopatterns.
SamenvattingZonder ons spierskeletstelse dat bestaat uit botten, gewrichten en spieren, zouden we niet kunnen overleven. Onze botten beschermen onze organen, geven structuur aan ons lichaam en ze maken het mogelijk dat we ons kunnen bewegen. Botcellen zorgen ervoor dat onze botten gezond blijven door kleine scheuren en breuken die veroorzaakt worden door dagelijkse activiteiten te herstellen. Helaas kan het voorkomen dat bottumoren verwijderd moeten worden of dat we ernstig verongelukken waardoor grote botdefecten ontstaan. Deze defecten zijn te ernstig om door onze botcellen hersteld te worden. In dit geval is een operatie nodig om de cellen te ondersteunen bij het botherstel. Botvervangers kunnen in het defect geplaatst worden om een brug te vormen tussen de twee uiteinden van het defect en zorgen ervoor dat cellen gestimuleerd worden om nieuw botweefsel te vormen.
De afmetingen van de beschikbare botvervangers voor de behandeling van botdefecten zorgen ervoor dat deze implantaten alleen in een defect geplaatst kunnen worden via een open operatie. Zo’n operatie veroorzaakt grote schade aan het lichaam wat leidt tot een langdurig herstelproces en het vergroot de kans op infecties. Minimaal invasieve chirurgie zou toegepast kunnen worden om de operatie minder ingrijpend te maken. Met deze techniek kunnen operaties uitgevoerd worden met speciale instrumenten die door kleine sneden in het lichaam worden gebracht. Om minimaal invasieve implantatie van botvervangers mogelijk te maken, zouden botimplantaten gemaakt moeten worden die door deze kleine openingen passen. Daarnaast is het bewezen dat het botherstel bevorderd kan worden en infecties voorkomen kunnen worden door specifieke nano-patronen op het oppervlak van een botvervanger aan te brengen. Helaas is het niet mogelijk om de technieken die hiervoor gebruikt worden toe te passen op de beschikbare botimplantaten vanwege hun drie-dimensionele structuur. Om deze twee problemen op te lossen zouden botvervangers uitklapbaar gemaakt kunnen worden en gevouwen kunnen worden vanuit een twee-dimensionele geometrie. Omdat uitklapbare en vouwbare botvervangers niet bestaan, is het doel van dit proefschrift om uit te zoeken of het mogelijk is om uitklapbare botvervangers te maken en deze te vouwen van vlakke platen.
In hoofdstuk 2 worden verschillende aspecten van de geometrie van een botvervanger onderzocht om erachter te komen hoe deze het botherstel beïnvloeden.
Ondanks de gewenste eigenschappen die de poreuze structuren in hoofdstuk 3 hebben, zijn ze niet geschikt om ze met minimaal invasieve technieken te kunnen implanteren. Daarom wordt een eerste stap gemaakt in de ontwikkeling van metalen uitklapbare botvervangers in hoofdstuk 4. In dit hoofdstuk worden mechanismen ontworpen die direct na hun fabricage met selective laser melting functioneel zijn. Dankzij scharnieren, verende elementen en staven kunnen deze mechanismen in- en uitgeklapt worden door op specifieke punten trek- en drukkrachten uit te oefenen.
De scharnieren die gebruikt worden voor de uitklapbare mechanismen in hoofdstuk 4 compliceren het ontwerp. Daarom worden in hoofdstuk 5 simpele structuren 3D-geprint die geen scharnieren bevatten maar op basis van elastische vervorming kunnen wisselen tussen twee verschillende stabiele configuraties. Deze simpele structuren kunnen op verschillende manieren samengesteld worden om uitklapbare structuren te vormen die meerdere stabiele configuraties hebben.
De structuren in hoofdstuk 5 kunnen ingeklapt en uitgeklapt worden, maar vanwege hun drie-dimensionele geometrie zijn ze niet geschikt om oppervlaktebehandelingen toe te passen. De kennis die we tijdens dit onderzoek hebben opgedaan is gebruikt voor de ontwikkeling van uitklapbare en vouwbare structuren die gepresenteerd worden in hoofdstuk 6. 3D-printen en het lasersnijden van metalen platen worden gebruikt om drie-dimensionele uitklapbare kubussen te maken. Dankzij de vlakke configuratie van de lasergesneden metalen platen konden micro-patronen aangebracht worden op het oppervlak. Ook kunnen de gesneden platen gevouwen worden om drie-dimensionele uitklapbare botvervangers te maken.
In hoofdstuk 7 worden de belangrijkste bevindingen van dit proefschrift besproken en worden de onderzoeksvragen uit hoofdstuk 1 beantwoord. Daarnaast worden er aanbevelingen gedaan voor toekomstige onderzoeken en alternatieve toepassingen voorgesteld.
Het werk dat gepresenteerd is in dit proefschrift is de eerste stap in de ontwikkeling van uitklapbare botvervangers en uitklapbare botvervangers die gevouwen kunnen worden van vlakke platen. We hopen dat onze ontwerpen inspireren voor de verdere ontwikkeling om botvervangers geschikt te maken voor minimaal invasieve chirurgie en oppervlaktebehandelingen toepasbaar te maken voor uitklapbare drie-dimensionele structuren.
1 IntroductionScience and art sometimes can touch one another, like two pieces of the jigsaw puzzle which is our human life, and that contact may be made across the borderline between the two respective domains. -M. C. Escher
Our bodies can be seen as magical worlds in which trillions of cells live and work together. These cells are responsible for many processes to make our organs and tissues function properly.
Our musculoskeletal system, which consists of bones, joints, and muscles, fulfils several important functions. For example, our bones are responsible for the support and protection of our organs while enabling our mobility. Therefore, it is important to keep them healthy. This is done by cells who repair small cracks and fractures caused by our daily activities. However, severe bone damage and large bony defects can occur due to different reasons, such as bone tumor resection or car accidents. In many such cases, the defects are too large for the cells to repair on their own and surgical intervention is required to support the bone regeneration process.
A bone substitute can be implanted into the defect to replace the lost bone and to act as a bridge between both parts of the native bone on either side of the defect. Cells are then able to move into the bone substitute to form new bone and to integrate the newly formed bone with the native bone. To ensure successful bone regeneration, it is important that the bone substitutes satisfy a long list of requirements, including biocompatibility and bioactivity, while also providing specific mechanical functions and favorable mass transport properties. Since this is not an easy task, many studies have been performed to develop bone substitutes, which fulfil those requirements.
1.2 Bone structure and the remodeling process
Bone is organized into multiple levels of structural hierarchy (i.e., macrostructure, microstructure, sub-microstructure, nanostructure, and sub-nanostructure ). At the macroscale, bone can be divided into cortical (or compact) bone and trabecular (or cancellous) bone [1, 2]. The stiffer and denser cortical bone can be found in 80% of a mature skeleton , while a combination of cortical and porous, spongy trabecular bone can be found in long and flat bones [1, 3, 4]. Cortical bone primarily consists of osteons, which are cylindrical structures that are aligned in parallel with the longitudinal axis of bones . Trabecular bone is made up of trabeculae, which are connected struts that form an efficient porous network to support the mechanical loads exerted on the bones [3-5].
Bone remodeling is required for the growth of the skeleton , to optimize the inner architecture of bones in order to support mechanical loads [3, 6], and to maintain calcium and phosphorous levels inside the body [2, 3]. The most important cells in this process are osteoclasts  and osteoblasts , whose roles are bone resorption and bone formation , respectively. In addition to those two cell types, osteocytes are crucial for a process called mechanotransduction [3, 6, 7]. This is a mechanism in which mechanical stresses are converted into biochemical signals. These signals are then used to regulate the osteoblast
ter 1 In
and osteoclast activity .
Although microdamage can be repaired by bone remodeling , the repair of large (i.e., critical size) bony defects, caused by accidents for example, require surgical intervention. As a rule of thumb, a defect is considered large when the length of the defect is 2-3 times the diameter of the bone involved . This means that, for example, defects larger than 3 cm in the bones of our lower arm, 5 cm in the bones of our legs, and 6 cm in the bone of our upper arm  cannot be repaired by our cells alone. Bone tissue engineering aims at the repair and regeneration of such large bone defects  by using biomaterials to integrate the newly formed bone w the native bone .
Bone substituting materials are used to fill large bony defects. Bone substitutes, such as autologous (from the same patient) and allogenic (from another person) bone tissue grafts are available. However, their limited supply [11-13], donor site morbidity [11, 13], and the risk of viral and bacterial disease transmission [11, 14] means that there is a need for engineered and innovative replacements [11, 12].
Synthetic replacements for bone grafts are called porous biomaterials. These biomaterials can be made of ceramics [7, 13], polymers [7, 13], or metals [15-18] and their alloys. They aim to help and guide our cells in the bone regeneration process . Biomaterials should be biocompatible so that they are not harmful for the cells and tissues in our body .
To make sure that our cells receive the nutrients and oxygen they require to survive and function as desired, the architecture of a biomaterial is important. Architectural parameters include the pore size [2, 21] and shape, the overall porosity of the biomaterial [2, 21], surface properties [2, 21], and mechanical properties [2, 21]. When the architecture is not optimal for the cells to live in, the bone regeneration process will be obstructed and the connection between the implant and the native bone will be too weak. The biomaterial remains or becomes loose and needs to be surgically removed and replaced. Therefore, a biomaterial should promote cells to become bone cells (osteoinduction) [7, 22], support bone growth (osteoconduction) [7, 22], and be able to integrate with the native bone (osseointegration) . The porosity, pore size, and the pore interconnectivity of bone substitutes are important to enable cells to travel through the biomaterial  and native bone and blood vessels  to grow into the porous structure. These events are necessary for the generation of de novo bone that integrates with the existing tissue.
The surface of a porous biomaterial is important, because the surface properties determine the cell response [7, 15]. Modifications to the surface, such as the application of nanopatterns [15, 23, 24] can induce cells to adhere to the surface, which is important for cells to travel through the implant (migration), to multiply (proliferation) [23, 24], and to specialize (i.e., differentiate) into the type of cells required for bone tissue regeneration [15, 24]. For bone implants, it is desired that the cells on the surface of the implant become bone cells. In addition to inducing bone formation, surfaces can be made antimicrobial [25, 26] to prevent serious infections, which can lead to implant failure.
3D printing or additive manufacturing (AM) has been recently used to manufacture complex and porous biomaterials [27-29]. Such biomaterials contain a large area of internal surfaces, which cannot be easily reached after fabrication. The main reason for this is that controlled surface patterning techniques can only be applied to flat surfaces [7, 30].
1.4 Minimally invasive surgery
Due to the dimensions and rigidity of available porous biomaterials, open surgery is commonly used for the treatment of large bone defects. A large incision is made to place the implant at the right location. This is a highly invasive process, which increases the risk of infections and is associated with long recovery times.
Minimally invasive surgery was introduced at the beginning of the 20th century . For
this type of surgery, incisions of 1 - 1.5 centimeters  are made to insert laparoscopic tools. Using these long cylindrical tools with a small camera, many treatments are performed on a daily basis. Minimally invasive surgery is applied to treat vascular diseases , to remove tumors from the brain , and to take biopsies . In addition to these examples, many other treatments have been performed using this surgery technique.
It is a challenging task to implant bone substitutes minimally invasively because biomaterials are in general rigid structures with large dimensions. Therefore, they cannot be deformed easily to fit through small incisions or to be placed at locations that are difficult to reach. To overcome these issues, biomaterials could be made deployable.
1.5 Deployable structures
Deployable structures are structures that, upon deployment, can change their configuration from a compact state to their operational configuration [36, 37]. This enables deployable structures to be transported in a compact way . Deployability is used for the transportation of antennas, solar panels, and masts into space , to carry an umbrella inside a bag , or to quickly place a temporary bridge to recover damaged infrastructures caused by natural disasters . Deployable structures can be designed using mechanical joints and rigid
ter 1 In
elements , elastic deformation, or plastic deformation.
1.5.1 Rigid assemblies
Rigid assemblies are deployable structures that consist of mechanical joints and rigid elements . An example of a deployable rigid assembly is an umbrella. An external force is required to change its configuration from retracted (closed) to deployed (open). A locking mechanism is integrated to keep the umbrella in its deployed configuration.
1.5.2 Elastic deformation
Deployable structures can also be made using elastic deformation. This kind of deformation happens in the elastic range of the material. Elastic deformations can be made undone when the external force is removed.
Elastic deformation can also occur in bi-stable and multi-stable structures, which have more than one stable configuration in which they are load-bearing. An external force is only required to elastically deform the structures locally to make them switch between the stable configurations.
1.5.3 Plastic deformation
In addition to elastic deformation, deployable structures can work on the basis of plastic deformation. Unlike elastic deformation, which enables a material or a structure to return to its original shape when the external force is removed, plastic deformation results in a permanent shape transformation. An example of deployable structures that are plastically deformed are stents used for coronary balloon angioplasty . Stents are placed inside a narrowed artery using minimally invasive surgery. A balloon may then be used to open the stent and to plastically deform the stent, thereby keeping the artery open .
To summarize, deployable implants can be made using mechanical joints and elastic deformation, which allow them to switch between different stable configurations. Plastic deformation on the other hand, can be used to deform structures or materials permanently.
1.6 Problem statement
The dimensions and rigidity of the available porous biomaterials for the treatment of large bone defects require implantation using open surgery. This may cause great damage to the body, resulting in a long recovery time for the patient and increasing the risk of infections.
Moreover, it has been demonstrated that the bone regeneration process can be improved by applying complex and precisely-controlled nanopatterns to the surface of
biomaterials, many surface patterning techniques cannot be used because they can only be applied to flat surfaces.
To resolve these two issues, porous biomaterials could be made deployable and be folded from a flat state to enable the application of minimally invasive procedures and the use of surface patterning techniques.
1.7 Aim and research questions
Because neither deployable nor foldable biomaterials have been developed before, the aim of this thesis is to explore the feasibility of making porous biomaterials deployable and foldable from a flat state. More specifically, the central research question addressed in this thesis is defined as:
Is it feasible to fold deployable biomaterials from a flat state which can be used for the treatment of large bone defects?
The following sub-research questions were addressed to answer the main research question: • What are the main requirements for bone substitutes in terms of their geometry,
mechanical properties, and mass transport properties and to what extent do existing designs and manufacturing techniques (e.g., 3D printing) achieve those properties? • How can mechanical joints and elastic deformation be used to develop deployable porous
• How can elastic deformation be used to develop deployable porous biomaterials? • How can deployable porous biomaterials be made foldable in order to apply precisely
controlled patterns to their surfaces?
In this thesis, different manufacturing techniques, materials, and designs were used and evaluated to explore the feasibility of making porous biomaterials deployable and foldable from a flat state.
1.8 Thesis outline
This thesis consists of seven chapters in total, including the Introduction (Chapter 1) and the General Discussion and Conclusion (Chapter 7). Chapter 2 and 3 adress the first sub-research question and each of the remaining chapters addresses one of the other sub-research questions.
To gain more knowledge about the important architectural parameters of porous biomaterials and their effect on the bone regeneration process, a literature review is
ter 1 In
presented in Chapter 2.
To evaluate the properties of rigid porous biomaterials of which the geometry can be fully controlled, four types of rigid porous biomaterials are presented in Chapter 3. These porous biomaterials were manufactured using selective laser melting (SLM), which is a 3D printing or additive manufacturing (AM) technique to build metal objects through in a layer-by-layer fashion. The fabricated biomaterials were evaluated in terms of their morphological, mechanical (both quasi-static and fatigue), and mass transport properties.
Although the porous structures presented in Chapter 3 offer unique combinations of mechanical and mass properties, they are not suitable to be implanted using minimally invasive procedures. Therefore, a first step towards deployable metallic biomaterials is made in Chapter 4. This chapter presents deployable non-assembly mechanisms, which were manufactured using SLM. Different geometries, including a bicapped cube, a bicapped square antiprism, and a bicapped trigonal antiprism, were designed and fabricated using a single-step fabrication process. This type of fabrication leads to the immediate functionality of the mechanisms after manufacturing. The structures consist of revolute joints, wavelike elements, and rigid rods. Moreover, they can be deployed and retracted when compressive and tensile forces are applied to some specific locations within the mechanisms.
The mechanisms presented in Chapter 4 include revolute joints, which complicate the design of deployable porous biomaterials. For this reason, elastic deformation was used to design multi-stable deployable structures in Chapter 5. In this way, revolute joints could be avoided to simplify the design. Bi-stable elements were manufactured using fused deposition modeling (FDM), which is an AM technique to fabricate polymer objects. The bi-stable elements were combined in various ways to make multi-stable structures, which can be deployed and retracted in different ways.
Although the bi-stable and multi-stable structures presented in Chapter 5 were deployable, their three-dimensional design did not allow for the application of surface patterns. The knowledge gained from the study in Chapter 5 was used for the development of the deployable and foldable structures presented in Chapter 6. FDM was used to manufacture panels with bi-stable elements, which were combined to assemble deployable cubes. In addition to these 3D printed structures, micromachining was used to cut unfolded cubes from metal sheets. Due to the flat state of the unfolded cubes, it was possible to apply micropatterns to their surfaces. Moreover, they could be folded into a 3D deployable cube. Silicone balloons were designed and manufactured to act as actuators for the deployment of the cubes.
Chapter 7 summarizes the most important findings of this thesis and tries to formulate succinct answers to the research questions presented in the introduction. Additionally, recommendations for future research are provided and alternative applications are proposed.
 J.-Y. Rho, L. Kuhn-Spearing, P. Zioupos, Mechanical properties and the hierarchical structure of bone, Medical engineering & physics 20(2) (1998) 92-102.
 A.R. Amini, C.T. Laurencin, S.P. Nukavarapu, Bone tissue engineering: recent advances and challenges, Critical Reviews™ in Biomedical Engineering 40(5) (2012).
 J.D. Black, B.J. Tadros, Bone structure: from cortical to calcium, Orthopaedics and Trauma (2020).  T.M. Keaveny, E.F. Morgan, G.L. Niebur, O.C. Yeh, Biomechanics of trabecular bone, Annual review of biomedical engineering 3(1) (2001) 307-333.
 C.H. Turner, Three rules for bone adaptation to mechanical stimuli, Bone 23(5) (1998) 399-407.  S. Tatsumi, K. Ishii, N. Amizuka, M. Li, T. Kobayashi, K. Kohno, M. Ito, S. Takeshita, K. Ikeda, Targeted ablation of osteocytes induces osteoporosis with defective mechanotransduction, Cell metabolism 5(6) (2007) 464-475.
 J. Mitra, G. Tripathi, A. Sharma, B. Basu, Scaffolds for bone tissue engineering: role of surface patterning on osteoblast response, Rsc Advances 3(28) (2013) 11073-11094.
 A. Salhotra, H.N. Shah, B. Levi, M.T. Longaker, Mechanisms of bone development and repair, Nature Reviews Molecular Cell Biology (2020) 1-16.
 E.F. Eriksen, Cellular mechanisms of bone remodeling, Reviews in Endocrine and Metabolic Disorders 11(4) (2010) 219-227.
 S. Stewart, S.J. Bryant, J. Ahn, K.D. Hankenson, Bone regeneration, translational regenerative medicine, Elsevier2015, pp. 313-333.
 C. Laurencin, Y. Khan, S.F. El-Amin, Bone graft substitutes, Expert review of medical devices 3(1) (2006) 49-57.
 Y. Yu, Y. Wang, W. Zhang, H. Wang, J. Li, L. Pan, F. Han, B. Li, Biomimetic periosteum-bone substitute composed of preosteoblast-derived matrix and hydrogel for large segmental bone defect repair, Acta biomaterialia 113 (2020) 317-327.
 M.M. Stevens, Biomaterials for bone tissue engineering, Materials today 11(5) (2008) 18-25.  C. Delloye, Tissue allografts and health risks, Acta orthopaedica Belgica 60 (1994) 62-67.
 A.I. Greer, V. Goriainov, J. Kanczler, C.R. Black, L.-A. Turner, R.M. Meek, K. Burgess, I. MacLaren, M.J. Dalby, R.O. Oreffo, Nanopatterned titanium implants accelerate bone formation in vivo, ACS applied materials & interfaces 12(30) (2020) 33541-33549.
 Y. Li, H. Jahr, K. Lietaert, P. Pavanram, A. Yilmaz, L. Fockaert, M. Leeflang, B. Pouran, Y. Gonzalez-Garcia, H. Weinans, Additively manufactured biodegradable porous iron, Acta biomaterialia 77 (2018) 380-393.
 Y. Li, J. Zhou, P. Pavanram, M. Leeflang, L. Fockaert, B. Pouran, N. Tümer, K.-U. Schröder, J. Mol, H. Weinans, Additively manufactured biodegradable porous magnesium, Acta biomaterialia 67 (2018) 378-392.
 Y. Li, P. Pavanram, J. Zhou, K. Lietaert, P. Taheri, W. Li, H. San, M. Leeflang, J. Mol, H. Jahr, Additively manufactured biodegradable porous zinc, Acta Biomaterialia 101 (2020) 609-623.
 T. Winkler, F. Sass, G. Duda, K. Schmidt-Bleek, A review of biomaterials in bone defect healing, remaining shortcomings and future opportunities for bone tissue engineering: The unsolved challenge,
ter 1 In
Bone & joint research 7(3) (2018) 232-243.
 L. Ghasemi-Mobarakeh, D. Kolahreez, S. Ramakrishna, D. Williams, Key terminology in biomaterials and biocompatibility, Current Opinion in Biomedical Engineering 10 (2019) 45-50.
 G. Turnbull, J. Clarke, F. Picard, P. Riches, L. Jia, F. Han, B. Li, W. Shu, 3D bioactive composite scaffolds for bone tissue engineering, Bioactive materials 3(3) (2018) 278-314.
 T. Albrektsson, C. Johansson, Osteoinduction, osteoconduction and osseointegration, European spine journal 10(2) (2001) S96-S101.
 L. Richert, F. Vetrone, J.H. Yi, S.F. Zalzal, J.D. Wuest, F. Rosei, A. Nanci, Surface nanopatterning to control cell growth, Advanced Materials 20(8) (2008) 1488-1492.
 J. Hasan, S. Jain, K. Chatterjee, Nanoscale topography on black titanium imparts multi-biofunctional properties for orthopedic applications, Scientific reports 7(1) (2017) 1-13.
 M. Ganjian, K. Modaresifar, M.R. Ligeon, L.B. Kunkels, N. Tümer, L. Angeloni, C.W. Hagen, L.G. Otten, P.L. Hagedoorn, I. Apachitei, L.E. Fratila-Apachitei, A.A. Zadpoor, Nature helps: Toward bioinspired bactericidal nanopatterns, Advanced Materials Interfaces 6(16) (2019) 1900640.
 J. Hasan, R.J. Crawford, E.P. Ivanova, Antibacterial surfaces: the quest for a new generation of biomaterials, Trends in biotechnology 31(5) (2013) 295-304.
 S. Arabnejad, R.B. Johnston, J.A. Pura, B. Singh, M. Tanzer, D. Pasini, High-strength porous biomaterials for bone replacement: A strategy to assess the interplay between cell morphology, mechanical properties, bone ingrowth and manufacturing constraints, Acta biomaterialia 30 (2016) 345-356.
 G. Campoli, M. Borleffs, S.A. Yavari, R. Wauthle, H. Weinans, A.A. Zadpoor, Mechanical properties of open-cell metallic biomaterials manufactured using additive manufacturing, Materials & Design 49 (2013) 957-965.
 J. Kadkhodapour, H. Montazerian, A.C. Darabi, A. Anaraki, S. Ahmadi, A. Zadpoor, S. Schmauder, Failure mechanisms of additively manufactured porous biomaterials: Effects of porosity and type of unit cell, Journal of the mechanical behavior of biomedical materials 50 (2015) 180-191.
 V.A. Bolaños Quiñones, H. Zhu, A.A. Solovev, Y. Mei, D.H. Gracias, Origami biosystems: 3D assembly methods for biomedical applications, Advanced Biosystems 2(12) (2018) 1800230.
 S.D.S. Peter, G.W. Holcomb III, History of minimally invasive surgery, Atlas of Pediatric Laparoscopy and Thoracoscopy (2008) 1.
 G. Li, S.K. Ling, H.A. Li, Y. Zhang, J. Hu, How to perform minimally invasive tibial cortex transverse transport surgery, Journal of Orthopaedic Translation (2020).
 D.L. Fischman, M.B. Leon, D.S. Baim, R.A. Schatz, M.P. Savage, I. Penn, K. Detre, L. Veltri, D. Ricci, M. Nobuyoshi, A randomized comparison of coronary-stent placement and balloon angioplasty in the treatment of coronary artery disease, New England Journal of Medicine 331(8) (1994) 496-501.  Y. Kim, S.S. Cheng, M. Diakite, R.P. Gullapalli, J.M. Simard, J.P. Desai, Toward the development of a flexible mesoscale MRI-compatible neurosurgical continuum robot, IEEE Transactions on Robotics 33(6) (2017) 1386-1397.
 S.H. Parker, F. Burbank, A practical approach to minimally invasive breast biopsy, Radiology 200(1) (1996) 11-20.
 A. Al Sabouni-Zawadzka, A. Zawadzki, W. Gilewski, Modern lightweight deployable engineering
 S. Pellegrino, Deployable structures, Springer2014.
 G. Kiper, E. Soylemez, Deployable space structures, 2009 4th International Conference on Recent Advances in Space Technologies, IEEE, 2009, pp. 131-138.
 I. Ario, M. Nakazawa, Y. Tanaka, I. Tanikura, S. Ono, Development of a prototype deployable bridge based on origami skill, Automation in construction 32 (2013) 104-111.
 G.P. Kumar, S. Yuan, F. Cui, P.S. Branicio, M. Jafary-Zadeh, Nanoglass-based balloon expandable stents, Journal of Biomedical Materials Research Part B: Applied Biomaterials 108(1) (2020) 73-79.
ter 1 In
The effects of the bone
substitute architecture on the
bone regeneration process
2 of bone substitute architecture on the bone regeneration process
The success of bone substitutes used to repair bone defects such as critical sized defects depends on the architecture of the porous biomaterial. The architectural parameters and surface properties affect the cell seeding efficiency, cell response, angiogenesis, and eventually bone formation. The relevant parameters include the pore size and porosity, pore shape and fiber orientation, surface properties, and mechanical properties. For example, small pores are preferable for cell seeding, but limit cell viability, cell proliferation and differentiation. Moreover, the pore size and geometry affect the alignment of cells and the structure of the regenerated bone. This chapter presents an overview of the effects of the architecture of a porous biomaterial on the cell seeding efficiency, cell response, angiogenesis, and bone formation.
This chapter was published as
Bobbert, F. S. L., & Zadpoor, A. A. (2017). Effects of bone substitute architecture and surface properties on cell response, angiogenesis, and structure of new bone. Journal of Materials Chemistry B, 5(31), 6175-6192.
Bone substitutes act as three-dimensional matrices that guide and promote bone regeneration in order to heal critical sized defects [1–3]. In these defects caused by trauma , tumor resection [4,5], or severe fracture [5,6], bone is unable to heal itself. The most common bone substitutes include autografts [7,8], allografts , and xenografts , which are pieces of bone removed from the body of the patient, another person, or an animal, respectively . Because the use of these biological grafts may result in damage to the body and their supply is limited, another solution has to be found . Therefore, new synthetic biocompatible porous materials are developed. These biocompatible materials could also be called biomaterials and are not harmful or toxic to living cells and tissues inside the body .
Depending on the biomaterial used (polymer, ceramic, or metal) (Table 1), different fabrication techniques could be applied to manufacture the designed porous biomaterials. For metal bone substitutes, selective laser melting (SLM) [10–16], selective laser sintering (SLS) , sintering , perforating titanium sheet  and capsule-free hot isostatic pressing (CF-HIP)  are some examples of the applicable production methods. Polymer and ceramic bone substitutes could be manufactured with porogen leaching [20–30], freeze drying , 3D printing of successive fiber/strut layers [32–36], electrospinning , or gas foaming [1,38]. The above-mentioned techniques vary in accuracy and the level of control
Table 1. Biomaterials abbreviations and material group.
Biomaterial abbreviation Full form of biomaterial Biomaterial group
CaP Calcium Phosphate Ceramic
HA Hydroxyapa�te Ceramic
MBG Mesoporous bioac�ve glass Ceramic
β-TCP β-tricalcium phosphate Ceramic
Ti6Al4V Titanium Metal
TiNi Titanium Nickel Metal
TT Trabecular �tanium Metal
CSNF Chitosan network ﬁbers Polymer
Col Collagen Polymer
CG Collagen-glycosaminoglycan Polymer
DEF diethyl fumarate Polymer
HFIP hexaﬂuoroisopropanol Polymer
PA polyacrylamide Polymer
PDMS poly(dimethylsiloxane) Polymer
PLGA Poly(lac�de-co-glycolide) Polymer
PPC poly(propylene carbonate) Polymer
PPF poly(propylene fumarate) Polymer
PCL poly(ε-caprolactone) Polymer
SF Silk ﬁbroin Polymer
SPCL Starch poly(ε-caprolactone) Polymer
TG thermoplas�c gela�n Polymer
TPU Thermoplas�c polyurethane Polymer
PDLLA poly(D,L-lac�c acid) Polymer
ter 2 The e
ffects of the bone sub
over the parameters that describe the architecture of the scaffold.
A lot of research has been undertaken to see how the architectural parameters and surface properties of a developed bone substitute influence the bone regeneration process. Parameters determining the performance of porous biomaterials for bone tissue engineering include pore size [39–43], pore shape [32,41,43], porosity [39,41,43,44], interconnectivity [39,42,43], fiber orientation , surface properties [2,39,45,46], and mechanical properties [39,40]. The design of biomimetic materials affects cell behavior and provides guidance during tissue regeneration. Therefore, the design parameters can be chosen such that the desired cell response is elicited and the formation and structure of the new bone is guided.
Bone formation occurs in several steps starting with cell seeding  or recruitment of stem cells. In the case of cell seeding, the cell seeding efficiency can be measured, which is the number or percentage of attached cells within the structure after a cell suspension is seeded . Cell viability is important in all stages of bone regeneration and depends on the availability of nutrients  and oxygen for the cells within a structure, as well as on waste removal .
Cells should be able to migrate and distribute throughout the structure to ensure a stable bone-implant fixation and bone formation within the structure. The migration of cells is a stepwise process. First, the lamellipodia and filopodia protrude at the front of the cell and adhere to the surface of the biomaterial, which is called focal adhesion . The cell pulls itself forward by releasing the adhesions at its back side and contracting its body . The strength of the focal adhesions influences the cell morphology  and is thought to determine cell response and gene expression [53–55].
During bone regeneration, cells proliferate and differentiate into osteoblasts which deposit a collagen matrix that becomes mineralized. The first stage (i.e., proliferation) takes place in the first days after seeding and consists mainly of cell division . During this stage, cells are still able to migrate . After proliferation, cells start to differentiate into osteoprogenitor cells until the end of the second week, and the release of alkaline phosphatase (ALP) increases [57,58]. In two weeks after the differentiation stage, osteocalcin (OCN) and osteopontin (OPN) are produced and secreted by the cells [57,58], indicating the presence of osteoblasts [57,58] (Table 2). When the collagen matrix is synthesized by osteoblasts , biomineralization is initiated and mineral crystals are formed within the collagen matrix . In parallel with the proliferation and differentiation of cells, blood vessels form from existing vessels (angiogenesis) . These vessels create a vascular network to provide oxygen and nutrients to the cells and developing tissue within the bone substitute . This network provides stem cells needed for bone regeneration and direct the differentiation of endothelial cells and pre-osteoblasts [61,62]. All these steps in the bone regeneration process and the architecture of the bone substitute determine the amount and the quality of the newly formed bone.
Understanding the effects of the architecture of a bone substitute on the cell response is important to optimize the design of porous biomaterials that are aimed for bone regeneration. This paper presents an overview of the effects of various architectural parameters and surface properties on the cell seeding efficiency, cell response, angiogenesis, and bone formation. The seeded cell types were mainly BMSCs, (pre) osteoblasts, and fibroblasts. Only in a limited number of cases the cell behavior seemed to depend on the type of seeded cells [63–65].
2.2 Pore size and porosity
Pores are the voids within a porous biomaterial which provide space where new tissue and blood vessels will grow [66,67]. The pore size (diameter of an individual void) and porosity (percentage of void volume within a porous biomaterial) are connected to each other when the bone substitute contains an interconnected pore network. An increase in pore size has been associated with an increased porosity in most studies. Increasing the porosity of a porous bone substitute is a way to lower the stiffness . This reduces the mismatch between the stiffness of a (metal) bone substitute and the host bone , thereby mitigating the problems associated with stress shielding .
The seeding efficiency (Table 3) depends on the number of attachment sites within a porous biomaterial and the available time for cells to attach to the surface . With an increased pore size, the surface area within the structure decreases, resulting in less attachment sites for the seeded cells [20,31]. In addition to the lower number of attachment sites caused by bigger pores and a higher porosity, the permeability of the porous biomaterial increases . A higher permeability value is associated with a higher flow rate, which reduces the time for cell attachment to the surface of the structure during seeding .
Marker abbreviation Full form of marker Expressed by
ALP Alkaline phosphatase Osteoprogenitor
RunX-2 Osteoprogenitor, osteoblast
OPN Osteopon�n Osteoblast
OCN Osteocalcin Osteoblast
OPG Osteoprotegerin Osteoblast, inhibits bone resorp�on
Col1 Collagen type 1 Organic matrix of bone, synthesized by osteoblasts
VEGF Vascular endothelial growth factor Growth factor blood vessels
BSP Bone sialoprotein Mineralized �ssue
Table 2. Osteogenic markers.
ter 2 The e
ffects of the bone sub
Several studies have shown that the seeding efficiency decreases as the pore size increases, regardless of the biomaterial or seeding cells used [1,12,38,44,71]. Cells are more likely to aggregate at the seeding surface of poly(e-caprolactone) (PCL) porous biomaterials with pores smaller than 84 μm . This results in an inhomogeneous distribution of cells throughout the structure . In structures with bigger pores (e.g., 116 μm), cells are able to penetrate the top surface and distribute homogeneously throughout the scaffold . However, when pores become larger (>162 μm), cells tend to escape from the structure . In a study by Salerno et al., PCL structures seeded with hMSCs with a bi-modal architecture (mean pore sizes 38 μm and 312 μm) and a mono-modal structure (mean pore size 325 μm) were compared . They found that cells distributed throughout the bi-modal scaffolds, but that they remained in the seeding region of the mono-modal scaffolds . Studies with silk fibroin (SF) scaffolds found a low seeding efficiency with no difference among scaffolds with pore sizes between 80 and 500 μm [22,23,72].
One explanation for this low seeding efficiency on these scaffolds is their high porosity which ranged between 71% and 96%. In general, small pores are preferable for cell seeding. However, these pores should be larger than 100 μm to make a homogeneous distribution throughout the porous biomaterial possible. Depending on the tortuosity of the void space, there is a limit to the pore size to prevent cell escape which will reduce the seeding efficiency.
Cell viability seems to be mainly affected by the pore size and the porosity of the biomaterial (Table 3). Different studies [1,12,20,31,44,72] found a higher cell viability in porous biomaterials with bigger pores, which can be related to the higher oxygen diffusion into the interior region of these structures . The oxygen diffusion within porous biomaterials with small pores is limited by cell aggregation at the surface and the low penetration level during cell seeding and migration. In decellularized bone scaffolds, no difference in cell viability was found for different pore sizes and porosities . The difference in these findings might be the result of the structure thickness, the pore size and porosity of these porous biomaterials, and the tortuosity of the void network. The porosity (and pore size) of different porous biomaterials varied between 71% and 94% (80–300 μm) (SF) , 36–58% (94–147μm) poly(lactide-co-glycolide) (PLGA) , 42–87% (500–1000 μm) (Ti6Al4V) , and for the decellularized bone substitutes between 70.4% and 88.3% (208–376 μm) . The lower cell viability in the SF  (Figure 2h) and PLGA  (Figure 2c) scaffolds with small pores can be explained by the pore size which was smaller than 100 μm.In these scaffolds, cells are more likely to aggregate and block the way for oxygen and nutrients to the center of the scaffolds. Based on these results, it could be concluded that pores smaller than 100 μm should be avoided to prevent cell death.
Po re s iz e an d po ro sit y Bi om at er ia l Se ed in g ce lls /im pl an ta �o n sit e Po re si ze [µ m ] (p or os ity [% ]) See din g e ﬃci enc y Cel l v iab ilit y Mig ra� on Alig nm ent Mor pho log y Pro life ra� on Ost eog eni c diﬀ ere n�a �on Ang iog ene sis Tiss ue for ma� on Min era liz a�o n Ref ere nce SF hM SC 11 2-22 4 ( 94 ) 40 0-50 0 ( 96 ) 11 2-50 0 ( 95 ) + + + 23 PC L L9 29 84 116 141 162 ++ ++ + - - - + + R 71 PL G A 3T 3 ﬁb ro bl as ts 94 (3 6) 12 3 (4 5) 14 7 (5 8) ++ + - + + ++ ++ + + S/ L S/ L S S S S+ - + ++ 1 SF BM SC 80 -1 50 ( 71 ) 15 0-20 0 ( 80 ) 20 0-25 0 ( 87 ) 25 0-30 0 ( 94 ) - - - - - + + + - + + + - + + + - + + + 72 SF hA SC 14 0 (7 6) 25 4 (8 7) + + + + + + + + + + B+ B+ + + 22 De ce llu la riz ed bo vi ne bo ne hE SC 20 8 (7 0) 31 5 (8 0) 37 6 (8 8) ++ + - + + + - ++ + - + + + + + B B+ B + + ++ 44 CG M C3 T3 85 120 325 - + ++ - - + - + ++ - + ++ 31 PL G A M C3 T3 10 0-30 0 10 0-40 0 10 0-50 0 - + ++ - + ++ - + + R S S - + ++ - + ++ 20 Ti 6A l4 V hP DC 50 0 10 00 + - - + - + - + 12 PC L + O M hB M SC 38 , 3 12 32 5 + - ++ + + - ++ + ++ * + + ++ 38 PD LL A M G 63 < 27 5 (8 7) < 32 5 (8 8) < 42 0 (8 5) - + + - + + L L/S S R S S - + ++ - + + C- C+ C+ - + + 24 PC L AS C 35 5-50 0 (6 5) 50 0-10 00 ( 65 ) 10 00 -1 50 0 (6 5) + + + B B/S S R/ E R/ E S + ++ ++ + ++ ++ - + ++ 73 PL G A – Ca P rB M SC /r at c al va ria l d ef ec t 47 0-59 0 ( 85 ) 59 0-85 0 ( 85 ) 85 0-12 00 (8 5) + + + + + ++ + - - B+ B B 26 PP F/ D EF BM SC >5 00 18 0-30 0 + - V+ V 21 Β-TC P /r ab bi t f as ci a lu m bo do rs al is 33 7 (7 3) 41 5 (7 4) 55 7 (7 1) 63 1 (7 2) - + + + F+ F F F 27 PL G A /R at p ro xi m al � bi a 10 0-30 0 ( 86 ) 30 0-50 0 ( 87 ) 50 0-71 0 ( 87 ) B B+ B + ++ + 81 Ti 6A l4 V /r at fe m or al d ef ec t 49 0 (8 8) 49 0 (6 8) B+ B 11 | Chap ter 2 The e
ffects of the bone sub
Cell migration depends on the pore size and porosity of a porous biomaterial (Table 3) [1,20,24,31,38,44,71,72]. Restricted cell migration was observed in porous biomaterials with small pores, while cells can migrate more easily and distribute homogeneously when a structure contains bigger pores up to 500 μm [20,31,44].
Cell alignment and morphology
Table 3 summarizes the results found on cell alignment and morphology (Figure 1). In large pores, cells tend to align with and form sheets on the pore walls [1,24,44,73] while cells are able to bridge smaller pores [69,73]. The sheet formation occurred in PCL scaffolds with pores between 1000 and 1500 μm .
In a study on Ti structures with a mean pore size of 425 μm, cells elongated and connected with other cells and the pore walls in pores whose size was between 100 and 150 μm . Pores larger than 200 μm could not be bridged and the cells aligned with the pore surface . No cell growth was found in pores smaller than 100 μm .
The sheet-formation of cells could be connected to a well-spread cell morphology [10,19,25,33,72,74] (Figure 1c–f) with filopodia adhered to different points on the pore surface, indicating strong focal adhesions [69,75]. These filopodia help the cell sheets to align within the pores . Cells that bridge small pores or several struts are subjected to higher strains than cells adhered to a single surface, depending on the ratio between the cell size and pore size or the distance between the struts . Cell sheets are formed by filopodia of cells that are connected to neighboring cells, leading to a better communication between the cells [77,78]. Furthermore, a close connection with the pore surface seems to improve the bone regeneration process . By modifying the pore size, the alignment within the pores and the cell morphology could be guided. However, the pore shape and biomaterial used should be taken into account as well.
a b c d e f
Figure 1: Cell alignment and morphology on different biomaterials with different surfaces and architectures. a) Spreading of BMSCs on surface of HA structures  b) BMSCs bridging several collagen fibers within the HA structure  c) spreading of osteoblasts and forming sheets on a convex surface in NiTi structures  d) osteoblasts adjusting morphology to the roughness of pores in NiTi structures  e) stretched morphology of BMSCs on MBG surface after 7 days  f) BMSCs show a well spread morphology and connecting to other MBScs after 7 days on MBG structures with a silk film created with a 5.0 % silk solution .
ter 2 The e
ffects of the bone sub
Cell proliferation depends on the amount of nutrients to produce a new cell and the available space for cells to grow and multiply [69,79]. The pore size and porosity are important to satisfy these requirements, resulting in higher proliferation rates in porous biomaterials with bigger pores and higher porosities [1,12,20,24,31,44,69,72,73] (Table 3). Porous biomaterials with large pores have more space for cell growth and enhance the diffusion of oxygen and nutrients. In the bi-modal and mono-modal PCL scaffolds mentioned before, the hMSCs within the seeding region of the mono-modal scaffolds proliferated faster than the cells within the bi-modal scaffolds up to 21 days after seeding . This was due to the higher availability of oxygen and nutrients at the top of the scaffolds compared to the center and the bottom of the scaffold . However, due to the high number of cells within the top part of these mono-modal scaffolds after three weeks, lack of space led to a reduction of living cells . A higher cell number was found within decellularized bone , SF , PLGA  and collagen–glycosaminoglycan (CG)  scaffolds containing more pores with a minimum size of 200–300 μm . Studies on PLGA-CaP  and SF  structures with pores between 140 and 1200 μm did not find a significant difference in cell proliferation. It is difficult to determine why some studies found a significant difference in proliferation and some did not. The materials (PLGA and SF) were used in the studies that found a significant difference in proliferation for larger pores as well as in studies that did not. Also, the pore sizes used in the latter studies were in the range of the pore sizes used in the studies in which pore size seemed to affect cell proliferation. And finally, the seeding cells used (ASCs and BMSCs) also do not seem to be the reason for the different findings. Therefore, it is not clear what pore size would promote cell proliferation.
The results in Table 3 imply that the pore size may affect cell differentiation. Studies on porous SF  and decellularized bone  structures found no significant difference in alkaline phosphatase (ALP) expression between structures with different pore sizes. However, an initially higher ALP activity was found in SF scaffolds (Figure 2h) with bigger pores . This might suggest that small pores delay osteogenic differentiation. Studies on poly (propylene fumarate) (PPF) , PLGA-CaP , PCL , poly (D,L-lactic acid) (PDLLA) , Ti6Al4V  and SF  scaffolds found an increased osteogenic differentiation in scaffolds with larger pores.
In a study on bi-modal and mono-modal PCL scaffolds, higher OPN levels were found at the top of the scaffolds with a mono-modal architecture . In those scaffolds, the seeded cells remained at the top of the scaffold and therefore faster proliferation and osteogenic differentiation occurred due to the high availability of oxygen and nutrients and exposure of the cells to osteogenic medium . One explanation that osteogenic differentiation
occurred more in large pores is that the cells tend to be more spread in large pores compared to small pores. This morphology is thought to promote osteogenic differentiation .
Blood vessel formation
Angiogenesis occurs by the formation of small branches at the ends of existing blood vessels  that grow into the bone substitute . The production of vascular endothelial growth factor (VEGF) is needed to stimulate the growth of these small blood vessels  and is found to be higher in porous PPF biomaterials (Fig. 2e) cultured in vitro with large pores (Table 3) . When insufficient blood vessels are present during the bone regeneration process, fibrous tissue will form . Fibrous tissue was found in porous biomaterials with small pores in an in vivo study on β-tricalcium phosphate (β-TCP) scaffolds . In the same study, more blood vessels with a bigger diameter were present and less fibrous tissue was formed in substitutes with pores bigger than 400 μm . It was also observed that porous biomaterials with pores between 470 and 590 μm contained more blood vessels as compared to porous biomaterials with pores larger than 590 μm . These results seem to suggest that pores larger than 400 μm are preferable for blood vessel formation and consequently for the delivery of oxygen and nutrients to the cells inside the bone substitute.
Figure 2: Different pore sizes, shapes and biomaterials. a. Ti6Al4V , b. SPCL , c. PLGA , d. BG , e. PPF , f. collagen-apatite , g. MBG , h. SF . a b c d e f g h | Chap ter 2 The e
ffects of the bone sub
Tissue formation and mineralization
Tissue formation and mineralization in porous biomaterials are affected by pore sizes and porosities (Table 3). In the initial stage (i.e., up to 2 weeks of in vitro culture), collagen structures were unorganized in a PDLLA structure . After this period, they became more complex and structurally organized . This was also found in implanted PLGA structures with a higher amount of collagen in structures with large pores compared to structures with small pores . Thicker collagen fibers were present in PDLLA scaffolds with medium sized pores compared to scaffolds with larger and smaller pores . Moreover, the amount of mineralized collagen was higher in scaffolds with medium sized pores compared to the scaffolds with large pores, and no calcium areas were found in scaffolds with the smallest pores (<275 μm) .
Porous biomaterials with larger pores were found to have a better and higher distribution of calcium and mineral deposition parallel to the pore walls in vitro . This could be an effect of the alignment of cells with the pore walls, higher cell viability, distribution, and proliferation rate in structures with large pores. An in vitro study showed increased bone formation in scaffolds with medium sized pores, which could be related to the higher number of osteoblasts present in the inner region of these scaffolds . Different in vivo studies have shown that a higher porosity promotes host bone ingrowth for a stable fixation with the bone substitute [11,70] and that larger pores suppress fibrous tissue infiltration . In an in vivo study by Sicchieri et al., most bone was formed in scaffolds with pores between 470 and 590 μm . The limited amount of fibrous tissue infiltration and high amount of bone formation in large pores seems to be related to the higher amount of space and blood vessels present in these structures. Therefore, it can be concluded that large pores and angiogenesis are important for bone formation.
Structure of the new bone
The structure of the new bone grown in vivo depends on the organization of the synthesized collagen, which seems to be affected by the pore size  (Table 3). It was observed that cells tend to align with the walls of big pores where they proliferate, differentiate, and synthesize a structured collagen matrix. When this matrix becomes mineralized, it forms a lamellar structure . Therefore, the alignment of cells with the pore walls in bigger pores could be used to control the structure of the newly formed bone. In a study on PLGA scaffolds with different pore size ranges of 100–300, 300–500 and 500–710 μm, the most newly formed bone with a lamellar structure was found in scaffolds with the medium pore size range .
2.3 Pore shape and fiber orientation
The geometry of pores within a bone substitute can be, among others, spherical, rectangular, square, hexagonal or trabecular-like, depending on the biomaterial and manufacturing process used (Figure 2). With solid freeform fabrication techniques, even more complex shapes can be realized (Figure 3) [82,83]. The pore size and shape affect the mechanical properties of porous biomaterials, as they determine the dimensions and orientation of the struts or fibers and, thus, the stress distribution inside those structural elements [12,13]. Moreover, stress concentrations due to the notches present inside the structure or caused by manufacturing imperfections could affect the mechanical behavior of porous biomaterials .
Scaffolds with a ladder-like structure and rectangular pores and scaffolds with large spherical pores collapse more easily than porous biomaterials with smaller uniform round pores . Studies on the mechanical properties of Ti6Al4V structures (Figure 3a) with different pore shapes (diamond, cube, truncated cuboctahedron, triangular, and hexagonal) showed different mechanical properties  and fatigue strength for different unit cells with a similar porosity .
In the studies evaluated (Table 4), not much research has been done on the seeding efficiency of different pore geometries. A study on SF scaffolds found no difference in the seeding efficiency of lamellar structures or structures with spherical pores . However, in a study
Figure 3. Selective laser melted Ti6Al4V porous biomaterials for bone regeneration based on triply periodic minimal surfaces . a. primitive, b. gyroid, c. I-WP, d. diamond
ter 2 The e
ffects of the bone sub